General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.36 g/cm³ Show Material materials with Density of 8.36 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa |

100.0 °C | 205 GPa Show Material materials with Elastic modulus of 205 GPa | |

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | |

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | |

400.0 °C | 186 GPa Show Material materials with Elastic modulus of 186 GPa | |

500.0 °C | 180 GPa Show Material materials with Elastic modulus of 180 GPa | |

600.0 °C | 173 GPa Show Material materials with Elastic modulus of 173 GPa | |

700.0 °C | 167 GPa Show Material materials with Elastic modulus of 167 GPa | |

Elongation | 100.0 °C | 48 % Show Material materials with Elongation of 48 % |

200.0 °C | 48 % Show Material materials with Elongation of 48 % | |

300.0 °C | 56 % Show Material materials with Elongation of 56 % | |

400.0 °C | 57 % Show Material materials with Elongation of 57 % | |

500.0 °C | 55 % Show Material materials with Elongation of 55 % | |

600.0 °C | 54 % Show Material materials with Elongation of 54 % | |

Unlock all property charts | ||

Tensile strength | 100.0 °C | 670 MPa Show Material materials with Tensile strength of 670 MPa |

200.0 °C | 630 MPa Show Material materials with Tensile strength of 630 MPa | |

300.0 °C | 620 MPa Show Material materials with Tensile strength of 620 MPa | |

400.0 °C | 605 MPa Show Material materials with Tensile strength of 605 MPa | |

500.0 °C | 595 MPa Show Material materials with Tensile strength of 595 MPa | |

600.0 °C | 580 MPa Show Material materials with Tensile strength of 580 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2 | 100.0 °C | 360 MPa Show Material materials with Yield strength Rp0.2 of 360 MPa |

200.0 °C | 330 MPa Show Material materials with Yield strength Rp0.2 of 330 MPa | |

300.0 °C | 290 MPa Show Material materials with Yield strength Rp0.2 of 290 MPa | |

400.0 °C | 280 MPa Show Material materials with Yield strength Rp0.2 of 280 MPa | |

500.0 °C | 275 MPa Show Material materials with Yield strength Rp0.2 of 275 MPa | |

600.0 °C | 270 MPa Show Material materials with Yield strength Rp0.2 of 270 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 100.0 °C | 1.43E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.43E-5 1/K | |

200.0 °C | 1.47E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.47E-5 1/K | ||

300.0 °C | 1.5E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.5E-5 1/K | ||

400.0 °C | 1.53E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.53E-5 1/K | ||

500.0 °C | 1.57E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.57E-5 1/K | ||

600.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

700.0 °C | 1.65E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1400 °C Show Material materials with Melting point of 1400 °C | Typical for Nickel Chromium Alloy | |

Specific heat capacity | 20.0 °C | 390 J/(kg·K) Show Material materials with Specific heat capacity of 390 J/(kg·K) | |

100.0 °C | 452 J/(kg·K) Show Material materials with Specific heat capacity of 452 J/(kg·K) | ||

200.0 °C | 462 J/(kg·K) Show Material materials with Specific heat capacity of 462 J/(kg·K) | ||

300.0 °C | 471 J/(kg·K) Show Material materials with Specific heat capacity of 471 J/(kg·K) | ||

400.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

500.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

600.0 °C | 495 J/(kg·K) Show Material materials with Specific heat capacity of 495 J/(kg·K) | ||

700.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 10.1 W/(m·K) Show Material materials with Thermal conductivity of 10.1 W/(m·K) | |

100.0 °C | 12.6 W/(m·K) Show Material materials with Thermal conductivity of 12.6 W/(m·K) | ||

200.0 °C | 14.3 W/(m·K) Show Material materials with Thermal conductivity of 14.3 W/(m·K) | ||

300.0 °C | 16 W/(m·K) Show Material materials with Thermal conductivity of 16 W/(m·K) | ||

400.0 °C | 17.7 W/(m·K) Show Material materials with Thermal conductivity of 17.7 W/(m·K) | ||

500.0 °C | 19.3 W/(m·K) Show Material materials with Thermal conductivity of 19.3 W/(m·K) | ||

600.0 °C | 21 W/(m·K) Show Material materials with Thermal conductivity of 21 W/(m·K) | ||

700.0 °C | 22.6 W/(m·K) Show Material materials with Thermal conductivity of 22.6 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m |

100.0 °C | 1.17E-6 Ω·m Show Material materials with Electrical resistivity of 1.17E-6 Ω·m | |

200.0 °C | 1.19E-6 Ω·m Show Material materials with Electrical resistivity of 1.19E-6 Ω·m | |

300.0 °C | 1.21E-6 Ω·m Show Material materials with Electrical resistivity of 1.21E-6 Ω·m | |

400.0 °C | 1.23E-6 Ω·m Show Material materials with Electrical resistivity of 1.23E-6 Ω·m | |

500.0 °C | 1.25E-6 Ω·m Show Material materials with Electrical resistivity of 1.25E-6 Ω·m | |

600.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

700.0 °C | 1.27E-6 Ω·m Show Material materials with Electrical resistivity of 1.27E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.05 % Show Material materials with Carbon of 0.05 % |

Chromium | 21 - 23.5 % Show Material materials with Chromium of 21 - 23.5 % |

Cobalt | 2.5 % Show Material materials with Cobalt of 2.5 % |

Copper | 1.5 - 2.5 % Show Material materials with Copper of 1.5 - 2.5 % |

Iron | 18 - 21 % Show Material materials with Iron of 18 - 21 % |

Manganese | 1 - 2 % Show Material materials with Manganese of 1 - 2 % |

Molybdenum | 5.5 - 7.5 % Show Material materials with Molybdenum of 5.5 - 7.5 % |

Nickel | 36.4 % Show Material materials with Nickel of 36.4 % |

Phosphorus | 0.03 % Show Material materials with Phosphorus of 0.03 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Tungsten | 1 % Show Material materials with Tungsten of 1 % |